The influence of ligand configuration, solvent size and solvent polarity on the porous shape and void volume in a series of isomeric or isomorphic porous MOFs
Huang, Wen-Huan; Luan, Xin-Jun; Zhou, Xiang; Chen, Jun; Wang, Yao-Yu; Shi, Qi-Zhen; CrystEngComm 15 (2013) 10389–; doi:10.1039/c3ce41801d

data_7214610
_publ_section_title
;
 The influence of ligand configuration, solvent size and solvent polarity
 on the porous shape and void volume in a series of isomeric or isomorphic
 porous MOFs
;
_journal_issue                   47
_journal_name_full               CrystEngComm
_journal_page_first              10389
_journal_paper_doi               10.1039/c3ce41801d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C43 H28 Mn2.5 O18'
_chemical_formula_weight         970.0
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 93.935(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.134(3)
_cell_length_b                   13.102(3)
_cell_length_c                   25.336(5)
_cell_measurement_temperature    296(2)
_cell_volume                     4349.6(16)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0014
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            9901
_diffrn_reflns_theta_full        27.45
_diffrn_reflns_theta_max         27.45
_diffrn_reflns_theta_min         1.61
_exptl_absorpt_coefficient_mu    0.795
_exptl_absorpt_correction_T_max  0.8362
_exptl_absorpt_correction_T_min  0.7474
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    1.481
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2760
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.17
_platon_squeeze_details
;
;
_refine_diff_density_max         3.606
_refine_diff_density_min         -1.459
_refine_diff_density_rms         0.142
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     574
_refine_ls_number_reflns         9901
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.026
_refine_ls_R_factor_all          0.0708
_refine_ls_R_factor_gt           0.0708
_refine_ls_shift/su_max          0.144
_refine_ls_shift/su_mean         0.005
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1336P)^2^+12.4995P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2185
_refine_ls_wR_factor_ref         0.2185
_reflns_number_gt                9899
_reflns_number_total             9901
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce41801d.txt
_cod_data_source_block           xb5884_0m
_cod_original_cell_volume        4349.7(16)
_cod_original_sg_symbol_H-M      P2(1)/n
_cod_database_code               7214610